2.
30 2 Mechanical Stress Order of Grain Boundaries
Crystal I Crystal II
Z
SII
Y
X
SI
Fig. 2.1 Diagram explaining how lattices of crystals I and II are generated from a reference system
XYZ by the transformations SI and SII, respectively
For a 2D distribution, this approach is equivalent to the Kröner generalized 3D
approach in which the continuous distribution of dislocations is expressed by a dis-
location density tensor α related to the β distortion by [3, 4]:
curl β = α (2.2)
The expression (2.1) reformulated by Christian in matrix notation leads to the
equation known as the Frank-Bilby equation that gives the Burgers vector density B
necessary to realise the compatibility at the interface between the crystals I and II:
B = (S−1
I − S−1
II ) · X (2.3)
SI and SII are afﬁne transformations that generate the lattices of crystals I and II
starting from a reference system (Fig.2.1), X is a vector of relatively large intensity
in the grain boundary plane and B is the Burgers vector content of all the dislocations
that are crossed by the vector X. If this equation is satisﬁed, the grain boundary is
free of long-range stresses.
Equation(2.3) is relevant for any interface but we focus here on grain boundaries.
For grain boundaries in cubic materials, a simple relation links the SI and SII
lattices to the rotation R between the crystals: R = SII.S−1
I . Equation(2.3) then
becomes equivalent to the 0-lattice equation in which I is the identity matrix:
B = (I − R−1
)X (2.4)
In Eqs.(2.3) and (2.4), B is not considered as the sum of discrete Burgers vectors
belonging to the crystal translation lattice or to the DSC lattice. Such a discretization
depends on the relaxation processes and is meaningless when the dislocation density
is very high (Fig.2.2).
B may be determined by using the Frank circuit drawn around the grain boundary,
equivalent to the Burgers circuit within the crystal (Fig.2.2). A vector X = XII,
traced in the grain boundary plane and indexed in lattice II, is obtained by applying
3.
2.1 Continuous Approach: The Frank-Bilby Equation 31
Fig. 2.2 Frank circuit: a
vector XI = XII is drawn in
lattice I, then surrounded by
a closed circuit starting and
ﬁnishing at the vector origin.
The same circuit is reproduced
around the grain boundary: it
starts at the extremity of XII
(vector in the grain boundary
plane obtained by the rotation
θ of the vector (XI) passes
through the origin O and
terminates at the extremity
of XI. This circuit displays
a closure failure B given by
Eq.(2.4) by substituting X for
XII
the rotation R to a vector XI in lattice I:
XI = R−1
XII.
In the cases of symmetrical grain boundaries, if a median lattice between the two
crystal lattices is considered as the reference system, then the I and II lattices are
deduced from this reference by equal and opposite rotations (± θ/2) around a ρ axis;
expression (2.4) takes the well-known form of the Frank formula:
B = 2 sin(θ/2)(X ∧ ρ) (2.5)
And provided that X is perpendicular to the rotation axis:
B = 2 sin(θ/2)|X| (2.6)
The absence of long-range stresses around the interface may be modelled by the
use of two continuous distributions of dislocations with Burgers vector densities of
opposite sign that cancel. One distribution may be regarded as an array of stress-
generator dislocations or coherency dislocations, the other as an array of stress-
annihilator dislocations or anti-coherency dislocations.For a detailed description of
this approach, the reader may refer to the book by Sutton and Ballufﬁ [8] and to the
articles by Olson and Cohen [9] and Bonnet [10, 11].
4.
32 2 Mechanical Stress Order of Grain Boundaries
2.2 Discrete Approach: The Read and Shockley Model
Studies of edge dislocation walls in a crystal, later recognised as a low-angle sym-
metrical tilt grain boundaries, developed about 20 years before the explicit structural
model of these grain boundaries due to Read and Shockley [7]. This model links the
grain boundary misorientation angle θ to the spacing d between the edge disloca-
tions of Burgers vector b that form a periodic network in the grain boundary plane
(Fig.2.3):
d =
b
θ
(2.7)
Fig. 2.3 Scheme showing
a low angle symmetrical tilt
grain boundary according to
Read and Shockley. The tilt
axis is perpendicular to the
plane of the ﬁgure
The classical Read and Shockley formula gives the intergranular energy in func-
tion of the misorientation angle, in the low-angle limit:
γθ = γθ θ(A − lnθ) (2.8)
γ0 = μb/4π(1 − ν) and A = b/2πr0 with μ, the shear modulus, ν the Poisson
coefﬁcient and r0 the dislocation core radius.
Equation(2.8) is easily obtained by summing the elastic energies of the N
edge dislocations (of unit length) contained in a unit area of the grain boundary
(N = 1/d). This calculation may be done provided the dislocations are sufﬁciently
far from each other (low θ angle) and the extension of the stress ﬁelds is equal to the
distance d. This equation, initially established for θ < 15◦, is fundamental. Indeed,
after having established their model, Read and Shockley predict its relevance for
high-angle grain boundaries formed by dislocations evenly spaced. In 1989, Wolf
proposed an empirical extrapolation of the Read and Shockley formula for high-angle
grain boundaries sharing the same mean plane, by substituting θ by sin θ [12].
In1947,LacombeandBeaujard[13]revealedtheexistenceofsub-grainboundaries
in aluminium single crystals owing to the preferential etching of the crystal surface
on the form of etch pit alignments. But no relationship was established between etch
pits and dislocations. In 1950, Read and Shockley suggested a correlation between
5.
2.2 Discrete Approach: The Read and Shockley Model 33
their model and the previous observations. It was only in 1953 that a proper veriﬁca-
tion of the validity of the dislocation model for sub-grain boundaries was obtained
on a germanium bicrystal by Vogel et al. [14].
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations
The Bollmann approach generalizes the Read and Shockley model of intergranular
dislocations at any grain boundary. It rests on Eqs.(1.23) and (1.24) that deﬁne the
O-lattice and the 02-lattice. The term intrinsic, which comes from the Latin intrin-
secus, indicates that these dislocations are inherent in the grain boundary structure
that cannot exist in their absence; they actually are structural dislocations.
2.3.1 Primary Intrinsic Dislocations
In the 0-lattice equation (I − R−1) xO = Bm, the Bm vector may always be con-
sidered as the sum of Burgers vectors bm of crystal I (subscript m for matrix).
Equations(1.23) and (1.22) for non-cubic materials) may be seen as the quantiﬁed
form of the Frank-Bilby Eq.(2.4) for grain boundaries in which x0 is a O-lattice
element. The different O elements are surrounded by Wigner-Seitz cell walls. The
intersections of the grain boundary plane with these walls form the b-net; they deﬁne
the lines of the geometrically necessary dislocations called primary intrinsic dislo-
cations (IGBD) localized in the regions of worse ﬁt between the two crystals. The
term primary indicates that these dislocations account for the deviation from the ﬁrst
invariant of the bicystal, i.e. the single crystal (θ = 0). The term secondary will be
used to explain the deviation from the second invariant, the CSL lattice.
The primary intrinsic dislocations possess a Burgers vector bm of the perfect
crystal dislocations and form a network with the same periodicity than the 0-lattice
(Fig.2.4). Their spacing decreases when the misorientation angle increases according
to the formula derived from the Frank Eq.(2.3) where |X|= d:
d =
bm
2sin θ/2
(2.9)
For low θ values, Eq.(2.9) is identical to the Read and Shockley expression (2.7).
The uniformly spaced distribution of the primary dislocations mathematically
predicted by Eq.(2.9) is generally not respected. Indeed, a spacing between two
dislocations must be physically compatible with the lattice period. Only the average
spacing measured on an arrangement of several dislocations meet this formula.
Let us illustrate the application of Eq.(2.4) to the prediction of the primary dislo-
cation content in a tilt grain boundary, then in a twist grain boundary, both displaying
a small misorientation θ = ε.
6.
34 2 Mechanical Stress Order of Grain Boundaries
Fig. 2.4 Diagram showing the localization of the primary intrinsic dislocations in a low angle tilt
grain boundary. A, B and O are nodes of the O-lattice. PI and PII (QI and QII) are homologous nodes
assimilated to one node. D represents a region of bad ﬁt where the primary dislocation is localized
• For a tilt grain boundary around [011] with θ = ε, cos ε # 1 and sin ε # ε. The
rotation matrix R between the crystals is:
R =
1 − ε ε
ε 1 0
− ε 0 1
(2.10)
I − R−1
=
0 − ε ε
ε 0 0
− ε 0 0
(2.11)
The indices of any vector in the (01−1) grain boundary plane are [xyy].
The product (I − R−1)X in Eq.(2.4) enables to deﬁne the three components of the
dislocation density vector B:
Bx = 0 By = εx Bz = − εx (2.12)
B is then perpendicular to the rotation axis and to the grain boundary plane (Fig.2.5)
Furthermore:
B = nbm and bm = a/2 [01 − 1]. (2.12bis)
The dislocations have an edge character.
There are exact solutions for relations (2.4) only for vectors X = x0 = [xyy]
such as:
x = ± bm/ ε x = ±2 bm/ ε x = ± n bm/ ε (2.13)
The X vectors cut the intergranular dislocations along [100], the dislocation lines
perpendicularto[100]inthegrainboundaryplaneareparallelto[011].Thelow-angle
tilt grain boundary is well described by edge dislocations parallel to the rotation axis
7.
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations 35
Fig. 2.5 Geometry of the
primary dislocation network
(b = a/2 [01−1]) in a low angle
[011] tilt grain boundary
and distant from d = b/θ, as predicted by Read and Shockley. In this description,
the distance between the dislocations is large as θ = ε is a very small angle.
We may also describe the low angle tilt boundary by using an equivalent rotation
between the crystals: θ = (ε +π), then cos (ε +π)# −1 and sin(ε +π) − ε. The
application of the previous procedure leads to predict the occurrence of dislocations
also parallel to the tilt axis but with a Burgers vector b = a [100]. Furthermore,
the distance between the dislocations is now very small ( θ = ε +π being large).
As an example, for a 2◦ misorientation in copper, the dislocations are distant from
about 7nm according to the ﬁrst description; they may be observed by conventional
transmission electron microscopy. According to the second description, the distance
is about 0.12nm and the dislocations are no longer individually distinguishable; the
physical reality of this description in terms of dislocations is questionable. Rather in
this case to use a continuous distribution of the deformation. It seems reasonable to
consider that the dislocation structure predicted by the ﬁrst description is likely to
be realised. This point will be discussed further.
Figure2.6 presents a primary dislocation network in a low-angle tilt grain bound-
ary (2◦ around 111) in a iron–molybdenum alloy with a b.c.c. structure [15].
The same approach for a low-angle twist grain boundary with a {001} plane results
in a structure composed of two screw dislocation networks perpendicular to each
other and with a Burgers vector b = a/2 110 ; the distances between the dislocations
Fig. 2.6 Electronic micro-
graph of a 2◦ 111 tilt grain
boundary in a Fe-1% Mo
showing a primary edge dislo-
cation network [15]
8.
36 2 Mechanical Stress Order of Grain Boundaries
Fig. 2.7 Electronic micrograph of a low-angle twist grain boundary θ# 4◦ around 001 , in gold
showing two primary screw dislocation networks aligned along the 110 directions (at 45◦ of g);
the spacing between the dislocations is d# 40nm [16]. Bubbles are artefacts (bad welded bicrystal
regions) resulting from the bicrystal manufacturing; disturbed parts of the network (as EF) indicate
the presence of extrinsic dislocations (see Sect.5.2)
agree with the experiments (Fig.2.7) [16]. As previously, other descriptions exist but
their physical meaning is questionable.
It must be stressed that, whatever the chosen description of a given grain boundary,
the dislocation content totally accounts for the rotation between the crystals: these
dislocations are geometrically necessary. But the adopted grain boundary structure
depends on the relaxations, and only the observation enables to specify what descrip-
tion is physically meaningful.
Besides, the distance between the dislocations decreases as the misorientation
increases and becomes so small that it is no longer compatible with the crystal lattice
periodicity; the dislocation stress ﬁelds then overlap. However, the O-lattice being a
continuous function of the misorientation, the primary dislocations must exist from
a strict geometrical point of view. This continuity is conﬁrmed by the observation
of an electron (or X-ray synchrotron) diffraction pattern of a grain boundary plane
[17]. Indeed, the periodic distribution of deformations in the plane constitutes an
optic grid; by selecting a diffraction spot, an electron microscopy image of the grid
may be obtained. The distance between the rows of this rebuilt network well satisﬁes
Eq.(2.9).
Insummary, theequationgivingthetotal dislocationcontent B inagrainboundary
is mathematically valid whatever the misorientation θ; but, for high θ values, it covers
the physical concept of dislocation density. Another discrete description of the grain
boundary structure is then proposed which refers to the second invariant of the
bicrystal, i.e. the CSL lattice.
9.
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations 37
2.3.2 Secondary Intrinsic Dislocation
As postulated by Bollmann, any grain boundary adopts as much as possible the struc-
ture of the neighboured coincidence grain boundary, provided relaxations on the form
of secondary intrinsic dislocations. These dislocations are localized in the regions
of bad ﬁt between the two DSC lattices of the coincidence grain boundary θc rotated
one with respect to other by an angle equal to the angular deviation between the real
and the coincidence grain boundaries. These lines correspond to the intersections of
the grain boundary plane with the walls of the O2-lattice predicted by Eq.(1.24).
The term secondary comes from the fact that these defects break the periodicity
of the primary dislocations. They form a sub-grain boundary in the grain boundary.
Then, coincidence grain boundary regions delimited by secondary dislocations con-
stitute the grain boundary (Fig.2.8).
Fig. 2.8 Schematic representation of the periodic arrangement of secondary dislocations (⊥) in
the primary network (⊥)
Conversely to the plurality of the primary dislocation structures for a given grain
boundary, only one secondary dislocation structure is predicted by Eq.(1.24). Indeed,
whatever the equivalent rotations chosen for the real and the coincidence grain
boundaries, the angular deviation matrix D is identical. However, different struc-
tures may exist for non-mathematical reasons, linked to the atomic relaxations in the
boundary.
The characteristics of the secondary dislocations depend on the tilt/twist character
of the deviation to the coincidence. In a tilt grain boundary, a pure tilt deviation may
exist either around the fundamental rotation axis or around another axis; otherwise
10.
38 2 Mechanical Stress Order of Grain Boundaries
the deviation may have a twist or mixed character. Depending on the case, the grain
boundary structure is constituted of only one secondary edge dislocation network
or of two screw dislocation networks or even several mixed dislocation networks.
Similarly, a twist grain boundary may present a twist, tilt or mixed angular deviation
to the coincidence. In any case, the dislocation lines correspond to the intersections
of the grain boundary plane with the O2-lattice walls.
The Burgers vectors of the secondary dislocations belong to the DSC lattice, but
are not necessarily the elemental vectors of this lattice. In order to determine the
Burgers vector of a secondary dislocation, a closed circuit drawn around the defect
in the grain boundary must be reproduced in the DSC lattice of the nearest coincident
grain boundary. A construction very useful for analysing the high-resolution trans-
mission electron microscopy images enables to determine the dislocation Burgers
vector and its associated step (Fig.2.9) [18]. A secondary dislocation provokes a
translation of the CSL lattice. A step vector s may be deﬁned, that relates an initial
coincidence node to the coincidence node obtained by translation. If the crystal I is
ﬁxed and the crystal II translated, then the step sIis deﬁned in the coordinate system
of crystal I; and reciprocally for sIIif the crystal II is ﬁxed. There are several choices
for the step vectors, related to each other by a DSC vector; the shortest one is usually
chosen. The height of the step associated to the dislocation is hI = sI n in crystal I
and hII = sII n in crystal II. It follows that:
b = sI − sII
h = n(sI + sII)/2 (2.14)
where n is the normal to the grain boundary plane (pointed from crystal I to crystal II).
The Burgers vectors of the secondary dislocations must be necessarily indexed in
the reference system of the bicrystal translation lattice (the DSC lattice). Otherwise,
if each vector si is indexed in the reference system of crystal i, we obtain the primary
Burgers vector of the defect.
Fig. 2.9 Construction in the DSC lattice of a = 5 grain boundary of three possible steps s, s and
s associated to a dislocation with vector ± b1. The empty and full symbols correspond to crystal
II and crystal I, respectively; the triangular symbols represent sites located at ± a/2 [100] along the
projection axis; a CSL in its original position; b Displacement of crystal II relative to crystal I by
a vector + b1; c displacement of crystal I relative to crystal II by a vector − b1 [18]
11.
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations 39
The average distance between the secondary dislocations is given by a formula
similar to (2.9)
d =
|bDSC|
2sin θ/2
(2.15)
This distance decreases when the coincidence index increases (|bDSC| decreases)
and/or when the angular deviation θ to the coincidence increases. As a result, the
dislocations cannot be experimentally distinguished beyond a certain value or
beyond a certain θ deviation from the neighbouring coincidence relationship. Fur-
thermore, with the diminution of |bDSC|, the contrasts associated to dislocations in
transmission electron microscopy decreases. Thus, while preserving an almost con-
stant spacing, the dislocations are less and less visible when increases. Figure2.10
illustrates this effect for a series of 001 twist grain boundaries in gold [19].
Fig. 2.10 Intrinsic secondary dislocation networks in 001 twist grain boundaries in gold showing
the diminution of their contrast when increases: a = 1, b = 0,289nm; b = 5, b = 0,129nm;
c = 13, b = 0,080nm; d = 17, b = 0,070nm [19]
12.
40 2 Mechanical Stress Order of Grain Boundaries
Figure2.11 presents a network of secondary dislocations in a tilt grain boundary
in nickel that totally account for the deviation θ = 0, 09◦ 112 of this boundary
with respect to the = 3 {111} coincidence grain boundary [20]. Dislocations A
are parallel to the 112 direction, their Burgers vector is the DSC vector of = 3
normal to the grain boundary plane, b = a/3 111 , and their distance (≈ 130nm) is
in good agreement with the calculated distance.
Fig. 2.11 Electronic micrograph in dark ﬁeld (crystal C2 is in extinction condition) showing a
network of intrinsic secondary dislocations (as A) in a near = 3 {111} tilt grain boundary in
nickel (B is an extrinsic dislocation that will be analysed in part II, Chap.5) [20]
The near one-dimensional coincidence grain boundaries displays a network of
secondary dislocations, the lines of which being parallel to the intersections of the
crystal planes in good ﬁt with the grain boundary plane.
In an approximate coincidence grain boundary, the structure in terms of dis-
location must account for the rotation and the deformation necessary to bring in
coincidence two multiple cells of the crystals. According to the choice of the rational
value of the (c/a)2 ratio that approximates the real value, these two components
(rotation and deformation) differ. Only the observed intergranular structure enables
to specify the relaxation mode chosen by the grain boundary. Let us consider a grain
boundary near the rhombohedral twin, often observed in alumina or hematite poly-
crystals. When the grain boundary plane is strictly parallel to the {01-12} twin plane,
the grain boundary is described by an exact bi-dimensional coincidence. But, most
often, the observed grain boundary deviates from {01-12}. Then, the grain boundary
is described in terms of tri-dimensional approximate coincidence, by reference to
speciﬁc rotations θ around (02-21) associated to rational values of (c/a)2 as close
as possible of the real value, (2.730)2 for alumina. The speciﬁc rotations with their
corresponding deformations ε for alumina are (Table2.1) [21]:
Table 2.1 Speciﬁc rotations
and associated deformations
giving rise to rational
coincidences for rational
values of the c/a ratio [21]
c/a θ◦ ε
7 2.739 85.90 0.003
29 2.728 86.05 0.001
36 2.730 86.02 0
13.
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations 41
The deformations decrease when increases, this is also true for hematite
(c/a = 2,733). Among the three previous descriptions, which is the one adopted by
the grain boundary: high coincidence index ( = 36) and zero deformation or small
coincidence index ( = 7) at the expense of a deformation? Only the experiment
enables to answer the question.
The DSC vectors of the different descriptions are such that the intensities of two
of them, b2 and b3, are almost identical whereas the third vector b1 decreases as
increases. A secondary dislocation network may be observed in a grain boundary,
the misorientation of which being close to that of the rhombohedral twin in alumina
(θ = 85◦5); the grain boundary plane is deviated by 8◦ from the rhombohedral plane
(Fig.2.12). The Burgers vector of the intrinsic dislocations have been identiﬁed as
a linear combination of the two almost identical vectors (b2 and b3), whatever the
grain boundary description. In that case, no approximate coincidence description
seems to be preferred. However, in a grain boundary with a plane very close {01-12}
in hematite, the secondary dislocations, observed by high-resolution transmission
electron microscopy, possess a Burgers vector that is the smallest DSC vector cor-
responding to a = 7 coincidence relationship [22].
Fig. 2.12 Network of intrin-
sic secondary dislocations C
in a grain boundary near the
rhombohedral twin in alumina
[21] (Extrinsic dislocations B
will be described in part II)
In the θ = 90◦ (10-10) grain boundaries that are numerous in tungsten carbide of
hexagonal symmetry, the secondary dislocations have Burgers vectors of the = 2
coincidence relationship with a deformation equal to 0.024 whereas another neigh-
boured description with a = 39 coincidence index only requires a 0.0016 defor-
mation [23]. Similar conclusions have been obtained for the (01-12) twin in zinc of
hexagonal structure. To decide what approximate coincidence is better adapted to
the grain boundary structure, the dislocation lines are determined; they correspond
to the intersections of the grain boundary plane with the O2-lattice associated to
the smallest coincidence index, = 13 in this case. But the description requires a
non-negligible deformation, about 0.5% [24].
Thus, in non-cubic system, the structure of a grain boundary close to different
approximate coincidences seems to adopt that of a grain boundary with a speciﬁc
rotation corresponding to the rational coincidence with the smallest index at the
expense of a larger deformation of the coincidence cell.
14.
42 2 Mechanical Stress Order of Grain Boundaries
2.3.3 Interest and Limit of the Intrinsic Dislocation Model
To sum up, intrinsic primary dislocations with Burgers vectors of the crystals describe
the low-angle grain boundary structures. Similarly, a high angle coincidence grain
boundary only contains primary dislocations, but the close spacing of these disloca-
tions does not give them any physical reality. Finally, a high-angle non-coincident
grain boundary contains primary dislocations accounting for the nearest coincidence
structureandsecondarydislocationsthataccommodatethedeviationbetweenthereal
and the coincidence grain boundaries. Most often, only the secondary dislocations
are visualized as the distances between the primary dislocations are too small.
Figure2.13 shows the evolutions of the expected dislocation spacing in function
of the misorientation angle θ and in function of the deviation θ from different coin-
cidences for 001 symmetrical tilt grain boundaries in gold [25]. The points reported
on the curves indicate the spacing experimentally determined on the conventional
transmission electron microscopy images. The smaller the coincidence index, the
larger the deviation θ authorized to visualize secondary dislocations.
Fig. 2.13 Evolution of the spacing d (in nm) in function of the misorientation θ of the dislocations in
001 symmetrical tilt grain boundaries in gold. The full line and the dotted lines give the spacing of
the primary and secondary dislocations, respectively. The points indicate in which grain boundaries
periodic dislocations have been observed [25]
The possibilities to simultaneously observe primary and secondary dislocations
are limited to few experiments; it was the case in gold for a [001] tilt grain boundary
deviated from about 1◦ from the nearest coincidence = 13 {320} (Fig.2.14).
The primary dislocations with Burgers vector a/2 [110] are distant from 0.77nm
(calculated distance 0.75nm) and the secondary edge dislocations with DSC Burgers
vector a/13 [320] are distant from 7nm, in agreement with the theoretical distance
of 7.1nm [25].
The Bollmann formalism does not claim to describe the physical reality of a
grain boundary, but constitutes a possible approach to knowledge. Bollmann himself
insists that the use of the 0-lattices only permits a discrete selection of the possible
15.
2.3 Bollmann’s Discrete Approach: Intrinsic Dislocations 43
Fig. 2.14 Electronic micrograph of a symmetrical [001] tilt grain boundary near = 13 {320} in
gold (g = 200). The ﬁne periodic contrasts are due to primary dislocations with Burgers vector a/2
[110], the large contrasts (arrows) are attributed to secondary dislocations with Burgers vector a/13
[320] [25]
displacement vectors B, characteristic of the continuous displacement ﬁeld of the
transformation A. It is a ﬁrst approximate model of linear relaxation in the grain
boundary plane where the fact that it is linear is pure convenience.
Moreover, whatever the expression used to describe the grain boundary structure
in terms of dislocations, Burgers vector density according to Frank-Bilby or discrete
dislocations according to Bollmann, there are a large number of transformations S
(or R) equivalent because of the symmetry operations of the crystals, i.e. depending
on the choice of the unit cell in the reference coordinate lattice. An example has been
given for the low-angle [011] tilt grain boundary (see Sect.2.3.1). The equivalent
matrices are obtained by multiplying SI, SII or R by a uni-modular matrix U corre-
sponding to an operation of the point group symmetry of lattices I or II. Thus, there
are a very large number of possible descriptions of the structure of a given grain
boundary. Bollmann favours a particular description called NNR for Nearest Neigh-
bour Relationship that corresponds to the minimal dislocation density by arguing
that it must be associated to an energy minimum (E proportional to b2) [26]. This
argument is based on the consideration of the long-range elastic strain ﬁelds, but
the local distortions due to intrinsic dislocations cancel at large distance. A grain
boundary at equilibrium only generates short-range strains; the strain distribution
depends on the intergranular relaxation modes and cannot be predicted by a geo-
metrical model. The Frank-Bilby and Bollmann equations are disconnected from the
grain boundary energy. Finally, a grain boundary is a unique physical object with a
precise structure and a precise energy. Among all the possible structures, none can be
selected a priori. This question will be discussed more thoroughly in the description
of grain boundaries constrained at triple junctions (see Sect.10.2.2) where it takes a
particular importance.
Despite its geometrical nature, the Bollmann model has been successfully applied
to identify intrinsic dislocations in numerous grain boundaries in different types of
materials. It is especially remarkable that periodic dislocations have been observed,
by high-resolution transmission electron microscopy, in symmetrical tilt grain
boundaries with high coincidence indices, as = 337 in silicon; in that case,
16.
44 2 Mechanical Stress Order of Grain Boundaries
the Burgers vectors of the intrinsic secondary dislocations do not correspond to the
elemental DSC vectors [27].
A dislocation network always reveals the existence of a preferred ordered state of
the grain boundary, whatever its description. The reason why a preferred state exists
is a subject of questioning in solid-state physics.
However, the high-coincidence index grain boundaries displaying periodic dislo-
cations are not true general grain boundaries; they generally display misorientations
around axes with simple indices and possess symmetrical grain boundary planes.
What happens for grain boundaries with random misorientations and asymmetrical
high index planes? These grain boundaries do not present dislocation networks at
the scale of the conventional electron microscopy and are not observable by high-
resolution electron microscopy. Do they obey a discrete or continuous description? A
partial answer to this question has been advanced when we deal with the grain bound-
ary structure at high temperature (See Sect.4.1), then with relaxation phenomena of
non-equilibrated grain boundaries (See Chap.9).
In summary, the dislocations predicted by Eqs.(1.23) and (1.24) are geometrically
necessary, but the actual dislocation content depends on the local intergranular stress
relaxations. The structure is governed by the energy minimization and any forecast
based on geometry alone cannot reﬂect reality. It is physics that determines the
real mode of relaxation and a physical description requires an atomistic approach
(Chap.3).
2.4 Partial Intergranular Dislocations
The grain boundaries may also contain partial dislocations, generally associated to
rigid body translations τ, thus not predicted by the geometrical formalism. Although
non-periodic, these dislocations belong to the grain boundary structure [28]. Their
Burgers vectors are determined by using the circuit mapping method proposed by
Pond [29]. This circuit is analogous to a Frank circuit but is drawn in the dichromatic
complex; it takes into account all the symmetry operations of the space group and
not only the translations. Partial dislocations may also result from the existence of
grain boundary structure variants. If regions of different structures along the grain
boundary are related by a symmetry operation, they are energetically degenerate.
Partial dislocations separating such regions have been observed in germanium [30]
and in a copper–silicon alloy [31]. Partial dislocations are often located at the junction
between two boundary facets, but may be also present in a straight part of the grain
boundary. They may result of the decomposition of the DSC intrinsic dislocations, as
observed in a = 3 {211} grain boundary where a perfect dislocation with Burgers
vector a/3 111 dissociates into two products with Burgers vectors a/9 111 and
2a/9 111 [28].
17.
2.5 Stress Fields Associated to Intrinsic Dislocations 45
2.5 Stress Fields Associated to Intrinsic Dislocations
The stress ﬁeld of a low-angle grain boundary has been calculated by Hirth and
Lothe, using isotropic linear elasticity and by adding the stress ﬁelds of the periodic
dislocations [32]. The dislocations are mixed; three components of their Burgers
vector (bx by bz) and thus three periodic networks are considered (Fig.2.15).
Fig. 2.15 The three periodic networks of dislocations that are considered to calculate the elastic
stress ﬁelds of a low angle grain boundary. The Burgers vector of the mixed dislocations is decom-
posed in two edge components along Ox (a), Oy (b) and one screw component along Oy (c) [32]
For a symmetrical tilt grain boundary constituted of egde dislocations with
Burgers vector bx, parallel to the z axis and distant from D along Oy (Fig.2.15a),
the stress components (in regions such as x D/2π) exponentially decrease with
the distance x from the grain boundary ; on the contrary the stress ﬁeld of an isolated
dislocation is inversely proportional to the distance from its line. The expressions of
the shear component σxy for the two types of defects may be compared:
• for a dislocation
σxy =
μb
2π(1 − ν)
x(x2 − y2)
(x2 + y2)
(2.16)
• for a tilt grain boundary
σxy =
μb
(1 − ν)
2πx
D
exp
−2πx
D
cos
2πy
D
(2.17)
where, μ is the shear modulus and ν the Poisson coefﬁcient.
The expression of σxx for the grain boundary is similar to that of σxy with
sin2πy/D instead of cos2πy/D. The value of x = 2D (y = 0), the shear compo-
nent of σxy due to the periodic arrangement, is about 1% of its value for an isolated
dislocation. In the grain boundary plane (x = 0) and for distances y < D/2π of a given
18.
46 2 Mechanical Stress Order of Grain Boundaries
dislocation in the network, more than 90% of the grain boundary stress σxxis due to
the dislocation at the origin. Midway between the two dislocations, the compression
stress of one dislocation is annihilated by the tension stress of the other. Then, there
is no long-range stress ﬁeld induced by a symmetrical tilt grain boundary. If now
we consider the stress ﬁeld due to a network of edge dislocations with a Burgers
vector by (Fig.2.15b), the component σyy does not cancel at long distance, in contra-
diction with the equilibrium condition given by Eqs.(2.3) or (2.4). The equilibrium of
the grain boundary imposes that there is no total Burgers vector parallel to the grain
boundary plane associated to edge dislocations. For the last component of the Burgers
vector bz (Fig.2.15c), the dislocations have a twist character. For a uni-dimensional
arrangement of dislocations parallel to Oz, the shear component σyz exponentially
tends to zero with the distance to the grain boundary, but the stress component σxz
preserves non-negligible values at large distance. A simple arrangement of screw
dislocations is then incompatible with the equilibrium condition (2.4). Equilibrium
in a pure twist grain boundary requires the formation of two screw dislocation net-
works perpendicular to each other that result in a rotation around the normal x; the
stress ﬁelds of these networks annihilate.
More generally, three dislocation networks with non-coplanar Burgers vectors
account for the misorientation of a random grain boundary. For a grain boundary
that satisﬁes the Frank-Bilby formula, the elastic stress ﬁeld analysis shows that the
combination of the three stress ﬁelds yields their annihilation, even if one of the
network generates long-range stresses. In the calculation, the elastic constants of the
crystals are used, whereas the elastic constants of the grain boundary may differ from
those of the crystals as found by simulation [33]. Although the elastic constant tensor
of a boundary is not known, these constants may strongly vary in the grain boundary
plane [34].
Another model for calculating the stress ﬁelds is based on the grain boundary
description in terms of disclinations [35]. On the contrary to the dislocation model,
it takes into account the disclination core energy and may apply to high-angle grain
boundaries (see Sect.3.5).
More complex situations than those previously described by Hirth and Lothe
have been addressed, in particular by considering no strictly periodic networks and
by studying the evolution of their stress ﬁelds during return to periodicity. These
approaches will be detailed in part II, Chap.9 when dealing with the return to equi-
librium of a non-equilibrated grain boundary.
To conclude, the knowledge of the elastic contribution is insufﬁcient to account
for the intergranular energy, we must know the contribution of the grain boundary
core. This constitutes the subject of the next session focussing on the grain boundary
atomic order.
19.
References 47
References
1. F.C. Frank, Symposium on the Plastic Deformation of Crystalline Solids (Ofﬁce of Naval
Research Pittsburgh, Pennsylvania, 1950), p. 150
2. B.A. Bilby, Report on the Conference on Defects in Crystalline Solids (The Physical Society,
London, 1955), p. 123
3. E. Kröner, in Statistical Continuum Mechanics (Springer, Berlin, 1972)
4. E. Kröner, in Physics of Defects, ed. by R. Balian, M. Kleman et J Poirier (North Holland,
Amsterdam, 1981), p. 219
5. W. Bollmann, Crystal Defects and Crystalline Interfaces (Springer, Berlin, 1970)
6. Bollmann, in Crystal Lattices, Interfaces, Matrices: An Extension of Crystallography ed. by
W. Bollmann (1982)
7. W.T. Read, W. Shockley, Phys. Rev 78(195), 275 (1950)
8. A.P. Sutton, R.W. Ballufﬁ, Interfaces in Crystalline Materials (Clarendon Press, Oxford, 1995)
9. G.B. Olson, M Cohen. Acta Metall. 27, 1907 (1979)
10. R. Bonnet, J. Phys. 43, C6–215 (1982)
11. R. Bonnet, Phil. Mag. A51, 51 (1985)
12. D. Wolf, Scripta Metall. 23, 1713 (1989)
13. P. Lacombe, L. Beaujard, J. Inst. Metals 74, 1 (1947)
14. H.E. Vogel, E.E. Thomas, Phys. Rev. 90, 489 (1953)
15. S. Lartigue, communication personnelle (1980)
16. L. Priester, R.W. Ballufﬁ, J. Microsc. Spectrosc. Electr. 4, 615 (1979)
17. S.L. Sass, T.Y. Tan, R.W. Ballufﬁ, Phil. Mag. 31, 559 (1975)
18. A.H. King, D.A. Smith, Acta Cryst. 36, 335 (1980)
19. T. Schober, R.W. Ballufﬁ, Phil. Mag. 21, 109 (1970)
20. S. Poulat, B. Décamps, L. Priester, Phil. Mag. A 77, 1381 (1998)
21. H. Grimmer, R. Bonnet, S. Lartigue, L. Priester L, Phil. Mag. A61, 493 (1990)
22. L. A Bursill, R.L. Withers, Phil. Mag. A 40, 213 (1979)
23. J. Vicens, E. Laurent-Pinson, J.L. Chermant, G. Nouet, J. Phys. 49, C5–271 (1988)
24. A.H. King, F.R. Chen, Phil. Mag. A 57, 431 (1988)
25. E.P. Kwan, R.W. Ballufﬁ, Phil. Mag. A 56, 137 (1987)
26. W. Bollmann, Mat. Sci. Eng. A113, 129 (1989)
27. J. Thibault, J.L. Putaux, A. Jacques, A. George, H.M.Michaud a et X. Baillin, Mat. Sci. Eng.
1164, 93 (1993)
28. R.C. Pond, Proc. R. Soc. Lond. A 357, 471 (1977)
29. R.C. Pond in Dislocations in Solids, vol. 8, ed. by F. Nabarro (North Holland, Amsterdam,
1989), pp. 1–66
30. J.J. Bacmann, G. Sylvestre, M. Petit, W. Bollmann, Phil. Mag. A 43, 189 (1981)
31. C.T. Forwood, L.M. Clarebrough, Phil. Mag. 47, 135 (1983)
32. J.P. Hirth, I. Lotte, Theory of Dislocations, 2nd edn. (McGrawHill, New York 1968), p. 671
33. D. Wolf, J.F. Lutsko, J. Mater. Res. 6, 1427 (1989)
34. A. Aber, J.C. Bassani, M. Khanta, V. Vitek, G.J. Wang, Phil. Trans. Roy. Soc. A339, 555 (1992)
35. V.Y. Gertsman, A.A. Nazarov, A.E. Romanov, R.Z. Valiev, V.I. Vladimirov, Phil. Mag. A59,
1113 (1989)
Be the first to comment